Temperature dependence of time-resolved photoluminescence in closely packed alignment of Si nanodisks with SiC barriers
© Kiba et al.; licensee Springer. 2013
Received: 4 April 2013
Accepted: 1 May 2013
Published: 10 May 2013
We study the temperature dependence of time-resolved photoluminescence (PL) in closely packed alignment of Si nanodisks (NDs) with SiC barriers, fabricated by neutral beam etching using bio-nano-templates. The PL time profile indicates three decaying components with different decay times. The PL intensities in the two slower decaying components depend strongly on temperature. These temperature dependences of the PL intensity can be quantitatively explained by a three-level model with thermal activation energies of 410 and 490 meV, depending on the PL components. The activation energies explain PL quenching due to thermal escape of electrons from individual NDs. This thermal escape affects the PL decay times above 250 K. Dark states of photo-excited carriers originating from the separate localization of electron and hole into different NDs are elucidated with the localization energies of 70 and 90 meV. In contrast, the dynamics of the fastest PL decaying component is dominated by electron tunneling among NDs, where the PL intensity and decay time are constant for temperature.
KeywordsTime-resolved photoluminescence Si nanodisks Neutral beam etching Bio-nano-templates
Attractive interdisciplinary research areas between electronic and photonic materials have been developed by modern semiconductor nanotechnology. Si nanostructures are particularly important because solar cells using Si have widely been investigated[1, 2], and optical interconnections among integrated Si circuits have also been proposed by developing Si-based photodiodes and optical modulators[3, 4]. Therefore, many types of Si nanostructures, such as nanocrystals (NCs), nanodots, and porous nanostructures, were reported by employing various fabrication processes[5–14]. Moreover, fabrication processes of the Si nanostructures using ‘top-down’ lithography techniques were strongly motivated for the purpose of applying the Si nanostructures to electronic and photonic devices.
We have recently proposed a fabrication process of Si nanodisk (ND) arrays, where the Si NDs are formed by damage-free neutral beam (NB) etching for Si thin films covered with etching masks of Fe nanoparticles which are regularly aligned by bio-protein engineering[15–20]. This fabrication process using the bio-templates enables us to prepare closely packed high-density Si NDs with the intentionally designed precise size and spacing in a nanometric scale with flexible film stacking. We have also observed intense photoluminescence (PL) emissions in a visible light region with fast decay times ranging from 10 ps to 2 ns. The fast decaying PL characteristics reflect the dynamics of photo-excited carriers in this high-density Si ND array system, in which wavefunctions of photo-excited carriers overlap among Si NDs to some extent, and the carriers can transfer among the NDs. Photo-generated or electrically injected carriers need to be effectively transferred among Si NDs for the optical applications to solar cells or light-emitting diodes. The spatial transfer of the carriers in nanostructures can also be affected by thermal effects, such as thermal hopping or escape. Therefore, in this paper, we investigate the detailed temperature dependence of time-resolved PL and the related carrier dynamics in these high-density Si ND arrays. Different types of PL quenching mechanism can be identified, and the activation energies for the PL thermal quenching are deduced from the temperature dependences of the PL intensity. The difference of the activation energy between different decaying PL components supports the existence of different wavefunctions of the carriers in this high-density ND system. The PL quenching phenomena elucidated in this study will give us useful information about the dynamics of photo-excited carriers, such as carrier separation and transport, when we apply these Si NDs to solar cells and high-speed photonic devices.
The high-density (7 × 1011 cm−2) Si ND arrays were fabricated from polycrystalline Si thin films deposited on thermally oxidized surfaces of Si substrates under ultra-high vacuum. Bio-nano-templates consisting of ferritin supramolecules containing Fe cores were used to prepare two-dimensional closely packed alignments of the Fe cores as etching masks on the surfaces of Si thin films. The size and interspacing of the Fe cores were intentionally designed by protein engineering for the ferritin supramolecules. The Si NDs were fabricated by forming SiO2 barriers around the Si NDs masked by the Fe cores using the NB etching and subsequent oxidation processes. Details of the fabrication process are described elsewhere[15–17]. The diameter, thickness, and interspacing distance of the Si NDs mainly used in this study were designed at 10, 4, and 2 nm, respectively, by the abovementioned ferritin-protein engineering. The capping and barrier layers of SiO2 were removed with NF3 treatment. Then, a 5-nm-thick SiC layer was finally deposited on the Si ND array under a high vacuum by sputtering.
The samples of the Si ND array were placed on a cold finger cooled by a closed He compressor in a vacuum cryostat with quartz windows. The time-resolved PL spectra were observed at various temperatures by combining the excitation of second harmonic femtosecond pulses with the wavelength of 400 nm, pulse width of 150 fs, and repetition rate of 76 MHz of a mode-locked Ti-sapphire laser, with the detection of a synchroscan streak camera (Hamamatsu Photonics, Hamamatsu, Japan). A spot diameter of the laser light focused on the sample surface was 100 μm. The excitation power density was 8.4 mJ cm−2. The number of electron–hole pair generated per one ND was calculated to be less than 1, taking the sheet density of ND into account. Therefore, the multiple exciton generation or Auger process were not induced. The time width of the instrumental response curve was less than 15 ps, and the time resolution of 5 ps was obtained after deconvolution with the instrumental response.
Results and discussion
Temperature dependences of the spectral shape and energy were not seen. Both PL bands exhibit similar temperature dependences of the intensity. The PL intensity of the E2 band is much weaker than that with the SiO2 barrier, which was previously reported. Therefore, we consider that this E2 band originates from oxygen-related surface or interface states of the Si NDs, and we would like to discuss mainly about the E1 emission. In the low-temperature regime below 150 K, the PL intensity is almost constant. The intensity increases toward 200 K and peaks at a maximum around 250 K. The PL intensity then decreases monotonically with further increasing temperature. Quantitative discussion about these temperature dependences of the PL intensity will be made later.
The transient PL for the E1 band emission as a function of temperature in the Si ND array is shown in Figure 1b. The temporal evolution of each PL profile cannot be expressed by a single exponential function. The best fit was obtained typically using a triple exponential function as shown in Figure 1c, which is common for all array samples of the high-density Si NDs. From this fitting, we have identified three PL decaying components with different time constants τ1 = 770 ps, τ2 = 110 ps, and τ3 = 15 ps, respectively, for this case at 250 K as an example. Several papers have demonstrated ultrafast PL in a sub-picosecond region for Si NCs by means of up-conversion PL. The ultrafast emission ranging 2.0 to 2.4 eV was observed, which was attributed to the pseudodirect gap emission from the core states of Si NCs[11, 12]. In contrast, the PL components observed in our samples show time constants ranging from 10 ps to 1 ns, where values are much higher than those of the above pseudodirect gap emissions. Therefore, the most probable origin of the E1 emission is emissive surface states weakly located at the interfaces of Si NDs. Dhara and Giri have reported the PL emission with the wavelength of about 600 nm with decay times of several nanoseconds. They assigned this PL to the quasi-direct bandgap emission in heavily strained Si NCs because of their unique preparation of the NCs by milling. Sa'ar reviewed recent developments in the PL studies of various Si nanostructures and suggested that neither quantum confinement model nor surface chemistry model can solely explain the entire spectrum of emission properties.
The three PL components with different decay times imply three different types of emissive sites in the present ND array. We assigned these three decaying components from the disk density and excitation power dependences of the PL decay time and intensity. The emission with the slowest decay time τ1 on the order of 1 ns was interpreted by electron–hole pairs or excitons localized at individual NDs, because this PL component was dominant in the case of low-density dispersive NDs with the disk interspacings larger than 40 nm. The emission with the decay time τ2 was understood by recombination of an electron–hole pair or exciton not strongly localized in each ND, where each wavefunction of the carrier spreads over neighboring NDs to some extent due to periodic regular alignment of the ND separated by ultrathin potential barriers. The fastest PL component with τ3 was attributed to the recombination which was strongly affected by the electron tunneling among the NDs. In other words, this fastest PL was quenched by the electron transfer. The latter two faster PL components appeared only at high excitation densities in the high-density ND arrays. The interpretation of the electron transfer was also supported by the conductance measurement for sister samples.
The Eact values, which express PL quenching slopes in the high-temperature region, were determined to be Eact1 = 490 meV and Eact2 = 410 meV for the time-resolved I1 and I2 components, respectively. The Eact values represent the energy difference between the emissive state E x and the transfer channel among NDs for thermally activated electron hopping. These values of Eact1 and Eact2 agree well with the barrier height of 0.44 eV for the electron, taking into account the SiC bandgap energy of 3.0 eV obtained from reflectance measurements of a thick SiC film fabricated by the same deposition method and the PL energy of 1.9 eV for the Si NDs. The valence band offset is assumed to be 0.6. The valence band offset for the Si/SiC interface has not been known as far as we know, but that of the Si/SiO2 has been recently determined to be 0.6. Therefore, we interpret that the obtained Eact values show a potential height for the electron at the Si ND/SiC interface. The difference in the above two activation energies (Eact1 − Eact2 = 80 meV) indicates the energy difference between the two emissive states showing the different decay times of τ1 and τ2, if we assume that the potential height responsible for the thermal escape is identical for both PL components. On the other hand, the Elow values, which describe negative quenching slopes of the gradual increases in the PL intensity at low temperatures, are obtained to be Elow1 = 70 meV and Elow2 = 90 meV for the time-resolved I1 and I2 components, respectively. At low temperatures, the electron and hole responsible for the I1 emission are separately trapped at different shallow potential minima within each ND, and the recombination rate significantly decreases. These spatially isolated electron and hole are thermally depopulated within the ND and can recombine at higher temperatures, which results in increases in the PL intensities. This lowest energy level is efficiently not emissive, but the carriers are not extinct via defect-related non-radiative centers because the thermally excited carriers from these states emit strong PL at higher temperatures.
The electron and hole responsible for the I2 emission can be localized at different NDs in the low-temperature regime and then the electron and hole pair is spatially separated. Therefore, the recombination probability decreases significantly (non-emissive). Increasing the temperature, the electron and hole are thermally excited to the free-like state (emitting I2), and the recombination of the electron and hole can take place again. We find that the Elow2 value indicating the activation (localization) energy of the I2 emission at low temperatures agrees well with the energy difference between Eact1 and Eact2; Eact1 (490 meV) − Eact2 (410 meV) = 80 meV (Elow2 = 90 meV). From this correspondence, we attribute the gradual increase in the I2 emission at the low-temperature region to the thermal excitation of the carriers from the dark state, where the electron and hole are localized in different individual NDs, to the free-like state among neighboring NDs.
At the lower temperature region below 200 K, the τnr value decreases with decreasing temperature, and the τPL becomes dominated by the τnr. This trend can be understood by the existence of non-emissive localized or trap states as discussed above. The τnr value increases toward the maxima with increasing temperature because of the thermal excitation of the carriers from the localized or trap levels to the emissive ones. In contrast, in the high-temperature regions toward room temperature, the τnr decreases with increasing temperature because of the thermal escape from the emissive level beyond the barriers. These PL dynamics for the two slower decaying PL components of I1 and I2, expressed by the temperature dependences of the τr and τnr, agree well with the thermal quenching and excitation processes elucidated by the temperature dependences of intensities of these PL components.
We have studied temperature dependences of time-resolved PL in the two-dimensional high-density Si ND arrays fabricated by NB etching using bio-nano-templates, where the PL time profiles with various temperatures are fitted by triple exponential decay curves. We find that the time-integrated PL intensities in the two slower decaying components depend strongly on temperature, which is attributed to PL quenching due to thermal escape of electrons from emissive states of individual NDs in addition to thermal excitations of carriers from localized or trap states in the individual NDs to the emissive ones. The temperature dependences of the PL intensity were analyzed by the three-level model. The following thermal activation energies corresponding to the thermal escape of the electron are obtained to 410 and 490 meV, depending on the PL components. In addition, we find dark states of photo-excited carriers, which can be attributed to the separate localization of the electron and hole into different NDs with the localization energies of 70 and 90 meV, depending on the PL components. The PL decay times of these two decaying components ranging from 70 to 800 ps are also affected by this thermal escape at high temperatures from 240 to 300 K. The fastest decaying component shows a constant decay time of about 10 ps for various temperatures, in which the decay characteristic is dominated by the electron tunneling among NDs.
This work is supported in part by the Japan Society for the Promotion of Science, Grant-in-Aids for Scientific Research (S) No. 22221007.
- Cho E-C, Park S, Hao X, Song D, Conibeer G, Park S-C, Green MA: Silicon quantum dot/crystalline silicon solar cells. Nanotechnology 2008, 19: 245201. 10.1088/0957-4484/19/24/245201View Article
- Conibeer G, Green M, Corkish R, Cho Y, Cho E-C, Jiang C-W, Fangsuwannarak T, Pink E, Huang Y, Puzzer T, Trupke T, Richards B, Shalav A, Lin K-l: Silicon nanostructures for third generation photovoltaic solar cells. Thin Solid Films 2006, 511–512: 654.View Article
- Bettotti P, Pavesi L: Nanosilicon: a new platform for photonics. Physica Status Solidi (c) 2011, 8: 2880–2884. 10.1002/pssc.201084114View Article
- Carreras J, Arbiol J, Garrido B, Bonafos C, Montserrat J: Direct modulation of electroluminescence from silicon nanocrystals beyond radiative recombination rates. Appl Phys Lett 2008, 92: 091103. 10.1063/1.2889499View Article
- Kůsová K, Cibulka O, Dohnalová K, Pelant I, Valenta J, Fučíková A, Zídek K, Lang J, Englich J, Matejka P, Štĕpánek P, Bakardjieva S: Brightly luminescent organically capped silicon nanocrystals fabricated at room temperature and atmospheric pressure. ACS Nano 2010, 4: 4495. 10.1021/nn1005182View Article
- de Boer WDAM, Timmerman D, Dohnalova K, Yassievich IN, Zhang H, Buma WJ, Gregorkiewicz T: Red spectral shift and enhanced quantum efficiency in phonon-free photoluminescence from silicon nanocrystals. Nat Nanotechnol 2010, 5: 878–884. 10.1038/nnano.2010.236View Article
- Valenta J, Fucikova A, Pelant I, Kůsová K, Dohnalová K, Aleknavičius A, Cibulka O, Fojtík A, Kada G: On the origin of the fast photoluminescence band in small silicon nanoparticles. New J Phys 2008, 10: 073022. 10.1088/1367-2630/10/7/073022View Article
- Xiaoming W, Dao LV, Hannaford P: Temperature dependence of photoluminescence in silicon quantum dots. J Phys D: Appl Phys 2007, 40: 3573. 10.1088/0022-3727/40/12/005View Article
- Trojánek F, Neudert K, Bittner M, Malý P: Picosecond photoluminescence and transient absorption in silicon nanocrystals. Phys Rev B 2005, 72: 075365.View Article
- Ray M, Hossain SM, Robert FK, Banerjee K, Ghosh S: Free standing luminescent silicon quantum dots: evidence of quantum confinement and defect related transitions. Nanotechnology 2010, 21: 505602. 10.1088/0957-4484/21/50/505602View Article
- Sykora M, Mangolini L, Schaller RD, Kortshagen U, Jurbergs D, Klimov VI: Size-dependent intrinsic radiative decay rates of silicon nanocrystals at large confinement energies. Phys Rev Lett 2008, 100: 067401.View Article
- Žídek K, Trojánek F, Malý P, Ondi L, Pelant I, Dohnalová K, Šiller L, Little R, Horrocks BR: Femtosecond luminescence spectroscopy of core states in silicon nanocrystals. Opt Express 2010, 18: 25241–25249. 10.1364/OE.18.025241View Article
- Dhara S, Giri P: Size-dependent visible absorption and fast photoluminescence decay dynamics from freestanding strained silicon nanocrystals. Nanoscale Res Lett 2011, 6: 320. 10.1186/1556-276X-6-320View Article
- Sa'ar A: Photoluminescence from silicon nanostructures: the mutual role of quantum confinement and surface chemistry. Journal of Nanophotonics 2009, 3: 032501–032542. 10.1117/1.3111826View Article
- Kubota T, Hashimoto T, Takeguchi M, Nishioka K, Uraoka Y, Fuyuki T, Yamashita I, Samukawa S: Coulomb-staircase observed in silicon-nanodisk structures fabricated by low-energy chlorine neutral beams. J Appl Phys 2007, 101: 124301–124309. 10.1063/1.2747226View Article
- Huang C-H, Igarashi M, Woné M, Uraoka Y, Fuyuki T, Takeguchi M, Yamashita I, Samukawa S: Two-dimensional Si-nanodisk array fabricated using bio-nano-process and neutral beam etching for realistic quantum effect devices. Jpn J Appl Phys 2009, 48: 04C187. 10.1143/JJAP.48.04C187
- Huang CH, Wang X-Y, Igarashi M, Murayama A, Okada Y, Yamashita I, Samukawa S: Optical absorption characteristic of highly ordered and dense two-dimensional array of silicon nanodiscs. Nanotechnology 2011, 22: 105301. 10.1088/0957-4484/22/10/105301View Article
- Huang C-H, Igarashi M, Horita S, Takeguchi M, Uraoka Y, Fuyuki T, Yamashita I, Samukawa S: Novel Si nanodisk fabricated by biotemplate and defect-free neutral beam etching for solar cell application. Jpn J Appl Phys 2010, 49: 04DL16. 10.1143/JJAP.49.04DL16
- Budiman MF, Hu W, Igarashi M, Tsukamoto R, Isoda T, Itoh KM, Yamashita I, Murayama A, Okada Y, Samukawa S: Control of optical bandgap energy and optical absorption coefficient by geometric parameters in sub-10 nm silicon-nanodisc array structure. Nanotechnology 2012, 23: 065302. 10.1088/0957-4484/23/6/065302View Article
- Kiba T, Mizushima Y, Igarashi M, Huang C-H, Samukawa S, Murayama A: Picosecond transient photoluminescence in high-density Si-nanodisk arrays fabricated using bio-nano-templates. Appl Phys Lett 2012, 100: 053117. 10.1063/1.3681793View Article
- Martin J, Cichos F, Huisken F, von Borczyskowski C: Electron–phonon coupling and localization of excitons in single silicon nanocrystals. Nano Lett 2008, 8: 656–660. 10.1021/nl0731163View Article
- Kiba T, Mizushima Y, Igarashi M, Samukawa S, Murayama A: Picosecond carrier dynamics induced by coupling of wavefunctions in a Si-nanodisk array fabricated by neutral beam etching using bio-nano-templates. Nanoscale Res Lett 2012, 7: 587. 10.1186/1556-276X-7-587View Article
- Igarashi M, Huang C-H, Morie T, Samukawa S: Control of electron transport in two-dimensional array of Si nanodisks for spiking neuron device. Appl Phys Express 2010, 3: 085202. 10.1143/APEX.3.085202View Article
- Shibata H: Negative thermal quenching curves in photoluminescence of solids. Jpn J Appl Phys 1998, 37: 550. 10.1143/JJAP.37.550View Article
- Seguini G, Schamm-Chardon S, Pellegrino P, Perego M: The energy band alignment of Si nanocrystals in SiO2. Appl Phys Lett 2011, 99: 082107. 10.1063/1.3629813View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.